Failure analysis of eleven Gates Glidden drills that fractured intraorally during post space preparation. A retrieval analysis study
Abstract The purpose of this study was to determine the failure mechanism of clinically failed Gates Glidden (GG) drills. Eleven retrieved GG drills (sizes #1 to #3) which fractured during root canal preparation were collected and the fracture location was recorded based on macroscopic observation. All fracture surfaces were investigated by a SEM. Then the fractured parts were embedded in acrylic resin and after metallographic preparation, the microstructure and elemental composition was evaluated by SEM and EDS. The Vickers hardness (HV) of all specimens was also determined. Macroscopic examination and SEM analysis showed that the drills failed near the hand piece end by torsional fatigue with fatigue cracks initiating at several locations around the circumference and propagating toward the center. Final fracture followed by a tensile overloading at the central region of cross section. Microstructural analysis, hardness measurements and EDS show that the drills are made of a martensitic stainless steel like AISI 440C. Based on the findings of this study, clinicians should expect fatigue fracture of GG drills that have small size during root canal preparation. Selection of a more fatigue resistant stainless steel alloy and enhancing the instrument design might reduce the incidence of quasi-cleavage fracture on GG drills.
Torsional and metallurgical properties of rotary endodontic instruments. 2. Stainless steel Gates Glidden drills.
A laboratory study was performed on stainless steel Gates Glidden drills to determine their torsional and metallurgical properties. Samples of #1 to #6 drills from the two manufacturers that distribute these instruments in the United States were tested in incremental and continuous clockwise torsional loading by using a digital torque meter. The values of mean torque at fracture obtained with these tests generally showed no statistically significant differences for the same drill size and a given manufacturer. However, it was not possible to completely evaluate drill sizes #5 and #6 because the torsional moments developed during testing exceeded the capacity of the test instrument. Scanning electron microscope examination confirmed the occurrence of ductile torsional fracture processes, which were evident from visual observation of the instruments after fracture. This study is part of a continuing investigation to establish standards for all rotary endodontic instruments.
Influence of filler addition, storage medium and evaluation time on biaxial flexure strength and modulus of adhesive systems
Abstract Objective. This study evaluated the effects of filler addition, storage medium and time on biaxial flexural strength and flexural modulus of six adhesive systems. Materials and methods. The adhesives were either unfilled resins: Single Bond, Prime&Bond 2.1 and One-Step; or filled resins: Single Bond Plus, Prime&Bond NT and One-Step Plus. Resin discs of each product (0.5 mm thick × 6.0 mm diameter) were prepared using silicon molds (n = 10). The discs were stored dry, in water, mineral oil or ethanol for 1 week or 3 months before biaxial flexural testing. Data were statistically analyzed by 3-way ANOVA and Tukey's post-hoc test (α = 0.05). The specimens were tested in a universal testing machine at 1.27 mm/min until failure occurred. Results. In general, the storage in ethanol led to significantly lower flexural strength and flexural modulus values than the other storage conditions for all adhesives in both storage periods. Filler addition increased flexural strength and flexural modulus for Prime&Bond NT, when it was stored dry or in water for 1 week. For Single Bond Plus, the filler addition resulted in higher flexural modulus, when it was stored for 1 week in oil and in ethanol. No significant differences in flexural modulus were observed between One-Step and One-Step Plus in any storage medium. Conclusions. Results suggested that filler addition does not necessarily have to increase the flexural strength and flexural modulus. Ethanol and oil storages tended to yield opposite effects.